Abstract cis-dichlorodiammineplatinum(II) (CDDP)-loaded polymeric micelles for cancer therapy have been developed to reduce the serious side effects of cisplatin CDDP. Herein, polymeric micelles incorporated with cisplatin are prepared based on the complexation between CDDP and hydrophilic poly (L-glutamic acid)-b-poly (2-methacryloyloxyethyl phosphorylcholine) (PLG-b-PMPC) diblock copolymers. These CDDP-loaded micelles possess an average size of 91 nm with narrow distribution, providing remarkable stability in media containing proteins. The release of CDDP from the micelles is faster at pH 5.0 and pH 6.0 than that at pH 7.4 and in a sustained manner without initial burst release. In addition, there is almost no difference in cellular uptake between these CDDP-loaded micelles and free CDDP. Moreover, in vitro cytotoxicity test shows they possess high efficacy to kill 4T1 cells as compared with free drug. Thus, PLG-b-PMPC copolymer might be a promising carrier for CDDP incorporating in cancer therapy. drug delivery, cisplatin, polymeric micelles, cancer therapy Introduction Cisplatin is an important class of antitumor drug and has been widely used for the treatment of many cancers, such as non-small cell lung carcinoma , ovarian cancer , testicular cancer  and gastric cancer . However, due to its severe dose-related side effects, i.e. neurotoxicity, nephrotoxicity, ototoxicity, nausea and myelosuppression [5–7], the clinical use of cisplatin is limited. Several cisplatin administration strategies and other platinum-based anti-tumor drugs have been used for reducing the disadvantages of cis-dichlorodiammineplatinum (II) (CDDP), which succeeded in less toxic but less efficacy [6–10]. Besides, the side effects are still the crucial barriers to increase dosage, which even result in irreversible renal failure . Therefore, considerable efforts have been dedicated for delivery systems that target platinum drugs to solid tumors to reduce the side effects while improving the efficiency of the drugs. Over the last two decades, the development of nanotechnology and the discovery of the enhanced permeability and retention (EPR) effect have provided powerful tools for drug delivery system (DDS) to reduce the side effects and improve the efficacy of antitumor drugs . The EPR effect has been demonstrated to enhance the accumulation of long-circulating macromolecules, which has facilitated the application of drug-loaded nanocarriers [13, 14]. Moreover, nanocarriers with suitable particle size (1 0–100 nm) and narrow size distribution can avoid rapid renal clearance by reticuloendothelial system (RES) . Nowadays, several kinds of CDDP-loaded nonocarriers, such as liposomes and polymer-platinum conjugates, have been develeped and even reached clinical trials . However, these fomulations are still defective by poor stability, low loading efficacy, weak solubility or undesired aggregation behaviour . To overcome these drawbacks, the strategies of assembling polymeric micelles by using block copolymers and cisplatin have been attractive to enhanced stability, superior blood half-life and tumor selectivity of CDDP-loaded nonocarriers [18–21]. Traditionally, polymers possess carboxyl groups have been investigated to incorporate cisplatin and form the hydrophobic core of micelles. Among them, polymeric micelles incorporating cisplatin prepared by Kataoka’s group via the polymer-metal complex formation between CDDP and poly(ethylene glycol)-b-poly (glutamic acid) block polymers have proceeded into clinical evalution [17, 22]. Although bioinspired poly (glutamic acid) with multi carboxyl groups is derived from naturally occurring glutamic acid, which is biocompatible and biodegradable . For the above CDDP-loaded micelles, hydrophilic PEG is usually used as shell-forming block to protect the drugs inside the core, prevent the interaction with plasma proteins and cells, avoid the recognition by macrophages and prolong the circulation in the bloodstream [24–27]. Besides conventional PEG, zwitterionic polymers containing phosphorylcholine are also attractive for their excellent hydrophilic, biomimetic property, outstanding biocompatibility, high antithrombogenic properties and remarkable resistant to protein adsorption [28–30]. For instance, poly (2-methacryloyloxyethyl phosphorylcholine) (PMPC) has been introduced into several nanocarriers as shell-building blocks for drug delivery [31–35]. Due to its membrane-mimetic structure, PMPC has been reported to be helpful for DDS in facilitating cellular association and enhancing cellular uptake [35, 36]. In our previous work, we had synthesized a poly (γ-benzyl-L-glutamate)-block-poly (2-methacryloyloxyethyl phosphorylcholine) (PBLG-b-PMPC) copolymer for drug loading, which showed great antitumor efficacy . However, the release of drugs was slow without stimuli-responsive property. Therefore, we hope to develop a more desirable drug carrier for quickly releasing the cargo in specific environment. In this work, hydrophilic poly (L-glutamic acid)-block-poly (2-methacryloyloxyethyl phosphorylcholine) (PLG-b-PMPC) copolymer is synthesized to complex with cisplatin, forming polymeric micelles as CDDP carriers through self-assembling (Scheme 1). The release of CDDP is controllable and shows a faster drug release at low pH. Additionally, these CDDP-loaded micelles possess an average size of sub-100 nm with narrow distribution, great protein stability, fast cellular uptake and also high tumor cells inhibition efficacy. Materials and methods Materials γ-benzyl-L-glutamate-N-carboxyanhydride (BLG-NCA, 97%, Chengdu Enlai biological technology Co., Ltd, China) was recrystallized twice from n-hexane/ethyl acetate (1/1, V/V) before using. 2-methacryloyloxyethyl phosphorylcholine was purchased from Nanjing Natural Science and Technology Institute and used without further purification. N-Boc-ethylenediamine, 2-Bromoisobutyryl bromide, 3-(4, 5-Dimethyl-thiazol-2-yl)-2, 5-diphenyl tetrazolium bromide (MTT), and 2,2′-Dipyridyl (bpy) were purchased from Chengdu Best Reagent Co., LTD (Chengdu, China) and used as received. Cuprous bromide (CuBr) from Chengdu Best Reagent Co., LTD (Chengdu, China) was purified by washing with acetic acid and ethanol. Cisplatin (CDDP) was purchased from Shanghai Ziyi Reagent (Shanghai, China). Extra dry N, N-Dimethylformamide (DMF) was purchased from Arcos Organics. All other reagents and solvents were purchased from Chengdu KeLong Chemical Reagent Company (Chengdu, China) and used without further purification. Synthesis of PLG-b-PMPC copolymers First, macroinitiator PBLG-Br was synthesized according to our previous report . Then, PBLG-b-PMPC copolymers were synthesized by ATRP method. Briefly, PBLG-Br (1 g, 0.2 mmol) and MPC (2.1 g, 7.0 mmol) were dissolved in a dry flask with 30 ml solvent (MeOH/DMSO, 1/1, v/v). After the oxygen was removed by a freeze-pump-thaw procedure for three times, CuBr (28.8 mg, 0.2 mmol) and 2, 2′-dipyridyl (62.4 mg, 0.4 mmol) were added into the flask under the atmosphere of N2. The reaction was performed for 48 h at 38°C with flame-sealed and the protection of N2. The reaction mixture was purified by passing through a silica gel column, concentrated, and precipitated into excess ethyl ether. The product was dried in vacuum at room temperature overnight. For the deprotection of the benzyl groups, PBLG-b-PMPC was dissolved in 0.1 M NaOH at room temperature for 1 h. The mixture was dialyzed against deionized water for 2 days. PLG-b-PMPC diblock copolymer was obtained by precipitating into excess amount of cold diethyl ether and followed by vacuum drying. Preparation of CDDP-loaded polymeric micelles Briefly, 20 mg PLG-b-PMPC and 4 mg CDDP were dissolved in 10 ml deionized water and stirred at 37°C for 72 h. CDDP-incorporated micelles thus prepared were purified by dialysis against deionized water for 24 h (MWCO 3500). The whole procedure was performed in the dark. The final volume of micellar solution was set to be 20 ml. The size distribution of the CDDP-loaded micelles was evaluated by a Malvern Zetasizer Nano ZS at 25°C. Drug loading content (DLC) and drug loading efficiency (DLE) were determined by inductively coupled plasma mass spectrometry (ICP-MS) and calculated by the following equations: DLC%=mass of loaded CDDPmass of the CDDP-loaded micelles×100% (1) DLE%=mass of loaded CDDPmass of CDDP used for loading×100% (2) In vitro drug release and micellar stability The release profiles of CDDP from CDDP-loaded micelles were evaluated by dialysis method. Typically, 2 ml CDDP-loaded micelles solution (1 mg/ml) was add to a dialysis bag (MWCO 3500) in 100 ml PBS solution and then incubated at 37°C in the dark. At predetermined time intervals, 2 ml solution were taken out from the release media and 2 ml fresh PBS was added into the release media. The released platinum was confirmed by ICP-MS. The stability of the micelles was evaluated by monitoring the particle size in 10, 20 and 50% (fetal bovine serum (FBS)/micellar solution, v/v) FBS over time. Cytotoxicity assay The cytotoxicity of PLG-PMPC copolymers, free CDDP and CDDP-loaded PLG-b-PMPC micelles against 4T1 cells were evaluated by the MTT assay. 4T1 cells were seeded in 96-well plates at a density of 5000 cells per well in 200 μl RPMI 1640 culture medium, which contained 10% FBS and supplemented with penicillin (50 U/ml) and streptomycin (50 U/ml) and incubated at 37°C in 5% CO2 atmosphere for 24 h. Then the culture medium was replaced by 200 μl fresh medium, which contained varying concentration of PLG-PMPC, free CDDP and CDDP-loaded micelles. The cells were incubated for another 48 or 72 h. But for free PLG-b-PMPC, the cells were incubated for another 24 h. At each time point, 20 μl MTT solution (5 mg/ml) was added to each well and incubated for 4 h at 37°C. Then the medium was replaced by 200 μl DMSO, followed by shaking for 20 min. The cell viability was measured in a Bio-Rad 680 microplate reader at a wavelength of 490 nm. The relatively cell viability was calculated by the following formula: Cell viability %=AsampleAblank×100% (3) where, Asample and Ablank referred to the absorbance of the sample wells and blank control wells, respectively. Data were presented as average ± SD (n = 3). Cellular uptake assay 4T1 cells were seeded in 24-well plates at a density of 5 × 104 cells per well in 500 µl RPMI 1640 culture medium and cultured for 24 h. The original medium was replaced by 450 µL fresh medium and 50 µl CDDP-loaded micelles solution (the concentration of Pt was 0.1 mg/ml) or free CDDP solution with the same concentration of Pt. The cells were incubated for 2, 4 or 6 h at 37°C. At each selective time, the culture medium was suck away, then the cells were washed three times with PBS before being treated with aqua regia (HCl: HNO3 = 3: 1, volume ratio) for 4 h. The solution was diluted to determine the Pt concentration by ICP-MS. Characterization 1H NMR spectra were recorded on a spectrometer operating at 400 MHz (Bruker AMX-400). The polydispersity of PBLG-Br were determined by gel permeation chromatography (GPC) (Agilent 1260). The measurements were performed using DMF as the eluent at a flow rate of 1 ml/min at 40°C and a series of narrow PMMA standards for the calibration of the columns. The GPC measurement of PLG-b-PMPC diblock copolymer was conducted on a water GPC system (Agilent PL aquagel-OH column, EcoSEC (HLC-8320GPC with distilled water as eluent (25°C, flow rate: 1 ml/min, and polyethylene glycol as standards). Transmission electron microscopy (TEM) measurements were performed on a Hitachi H-600 transmission electron microscope with an accelerating voltage of 100 KV. A drop of the micelle solution (1 mg/ml) was deposited onto a 230 mesh copper grid and treated with 2% phosphotungstic acid at pH 6.5 negative stain solution, then allowed to dry at room temperature before measurements. Inductively coupled plasma mass spectrometry (ICP-MS, VG PQExCell, Thermo Jarrell Ash, USA) was used for determined the quantity of CDDP. Results and discussion Synthesis of hydrophilic PLG-b-PMPC copolymers The synthetic route of PLG-b-PMPC was shown in Scheme 2. PBLG-Br macroinitiator was synthesized and its 1H NMR result was shown in Fig. 1A. The molecular weight distribution of PBLG-Br macroiniator was determined by GPC to be 1.22 (Fig. 2A). Amphiphilic PBLG-b-PMPC copolymers were obtained by ATRP of MPC using PBLG-Br as the initiator. The 1H NMR result of PBLG-b-PMPC was shown in Fig. 1B. When compared with Fig. 1A, characteristic peaks of PBLG (δ 7.34, –C6H5; δ 5.07, –CH2-C6H5) and characteristic peaks of PMPC (δ 4.27, -CH2-OC = O-; δ 4.17, -CH2CH2-OC = O-; δ 4.02, -CH2-CH2-N+(CH3)3; δ 3.71, -CH2-N+(CH3)3; δ 3.28, -N+(CH3)3) were found, suggesting the successful synthesis of PBLG-B-PMPC copolymer. Finally, hydrophilic PLG-b-PMPC copolymers were obtained by the deprotection of benzyl groups in NaOH solution. Obviously, Fig. 1C displayed that the benzyl group signals located at δ 7.34 ppm and methylene located at δ 5.07 ppm disappeared after the deprotection. Although the characteristic peaks of PLG-b-PMPC (δ 2.16, -CH2COOH; δ 1.96, -CH-CH2-; δ 4.23, -CH2-OC = O-; δ 4.15, -CH2CH2-OC = O-; δ 4.02, -CH2-CH2-N+(CH3)3; δ 3.61, -CH2-N+(CH3)3; δ 3.17, -N+(CH3)3) were found, indicating that the deprotection was complete. Furthermore, the DP of the PLG segment was calculated to be 21 based on the ratio of integration at peak b (-CH2-COO-, 2 H) and peak c (-CH2-COOH, 2 H) in Fig. 1C. Although the DP of the PMPC segment was calculated to be 34 based on the ratio of integration at peak b(-CH2-COO-, 2 H) and peak h (-CH2N+(CH3)3, 2 H). Therefore, the PLG-b-PMPC that we studied in this work can be defined as PLG21-b-PMPC34 with the molecular weight of about 12 700 g·mol−1 based on the 1H NMR result. The molecular weight of PLG-b-PMPC was further determined as 16 400 g•mol−1 by GPC with a PDI of 1.2 (Fig. 2B). Scheme 1. View largeDownload slide Schematic illustration of self-assembly of cisplatin-loaded PLG-b-PMPC polymeric micelles Scheme 1. View largeDownload slide Schematic illustration of self-assembly of cisplatin-loaded PLG-b-PMPC polymeric micelles Scheme 2. View largeDownload slide Synthetic route of PLG-b-PMPC Scheme 2. View largeDownload slide Synthetic route of PLG-b-PMPC Figure 1. View largeDownload slide 1H NMR Spectra of PBLG-Br (A) in DMSO-d6, PBLG-b-PMPC (B) in CD3OD and DMSO-d6 (1/1, V/V) and PLG-b-PMPC (C) in D2O Figure 1. View largeDownload slide 1H NMR Spectra of PBLG-Br (A) in DMSO-d6, PBLG-b-PMPC (B) in CD3OD and DMSO-d6 (1/1, V/V) and PLG-b-PMPC (C) in D2O Figure 2. View largeDownload slide GPC Trace of PBLG-br macroinitiator in DMF (A) and PLG-b-PMPC diblock copolymer in water (B) Figure 2. View largeDownload slide GPC Trace of PBLG-br macroinitiator in DMF (A) and PLG-b-PMPC diblock copolymer in water (B) Preparation and stability of CDDP-loaded PLG-b-PMPC polymeric micelles As shown in Scheme 1, CDDP-loaded PLG-b-PMPC polymeric micelles could be prepared by complexing cisplatin with carboxylate groups of the PLG segment. The average size of these CDDP-incorporated micelles was measured by DLS, which was 91 nm with a narrow distribution of 0.10 ± 0.04 (Fig. 3A). In the TEM image, the result revealed the well formation of these CDDP-loaded micelles (Fig. 3B). The average diameter of the micelles in TEM image was around 43 nm which is smaller than that scaled by DLS, which might due to the dehydration of the PMPC shell during the sample preparation process for TEM. The DLC and drug loading efficacy (DLE) of Pt determined by ICP-MS were 14.8 and 86.5%, respectively, based on the CDDP/polymer feed ratio of 20%. Figure 3. View largeDownload slide (A) The Size distribution of CDDP-loaded micelles with a PdI of 0.1 ± 0.04; (B) TEM image of CDDP-loaded micelles; (C) Particle size of CDDP-loaded micelles incubation with differents concentrations of FBS (FBS/micellar solution, v/v) at 37 °C as measured by DLS. The data were presented as the average ± SD (n = 3); (D) Accumulative release of CDDP-loaded micelles in PBS (pH = 5.0, 6.0 and 7.4). All measurements were carried out in triplicate. The data were presented as the average ± SD (n = 3) Figure 3. View largeDownload slide (A) The Size distribution of CDDP-loaded micelles with a PdI of 0.1 ± 0.04; (B) TEM image of CDDP-loaded micelles; (C) Particle size of CDDP-loaded micelles incubation with differents concentrations of FBS (FBS/micellar solution, v/v) at 37 °C as measured by DLS. The data were presented as the average ± SD (n = 3); (D) Accumulative release of CDDP-loaded micelles in PBS (pH = 5.0, 6.0 and 7.4). All measurements were carried out in triplicate. The data were presented as the average ± SD (n = 3) It was well known that the protein adhesion onto the drug carrier surface was one of the most important biological barriers that not only induced undesirable aggregation but also caused recognition by RES system, in which drug carriers would be rapidly cleared out of blood circulation . In this study, one of the purpose to introduce biomimetic PMPC as micelle shell was to enhance the protein resistence of the DDS due to its zwitterionic structure. To investigate the stability of CDDP-loaded micelles, micellar solution (1 mg/ml) was incubated with 10, 20 and 50% FBS for up to 24 h, and the particle sizes were monitored by DLS. As shown in Fig. 3C, there was almost no change in the particle size of CDDP-loaded micelles with 10% FBS. Meanwhile, the particle size of CDDP-loaded micelles solution with 20 or 50% FBS only had a slight change, which indicated the great stability of CDDP-loaded micelles in biological solution. In vitro release behavior of CDDP from CDDP-loaded PLG-b-PMPC micelles The in vitro release behavior of CDDP from CDDP-loaded PLG-b-PMPC micelles was investigated in PBS with pH 7.4, 6.0 and 5.0, respectively. It has been reported that CDDP-incorporated micelles could dissociate into unimers with CDDP release in chloride ion-rich solutions due to an inverse ligand substitution of the Pt (II) atom from the PLG segments to chloride. Moreover, cisplatin was usually released faster from these micelles under acidic condition than that at physiological condition due to the protonation of the carboxylic groups . As shown in Fig. 3D, cisplatin was released in a sustained manner without initial burst release and the release of cisplatin at pH 5.0 and pH 6.0 were faster than that at pH 7.4, which was beneficial for drug release specifically in tumor tissue with acidic enviroment. Cellular uptake and cytotoxicity of CDDP-loaded PLG-b-PMPC micelles The cellular uptake of CDDP-loaded PLG-b-PMPC micelles was quantified by ICP-MS with high detection sensitivity, and free CDDP was used as control. As shown in Fig. 4, the cellular uptake of the CDDP-loaded micelles was similar with free CDDP within 6 h, suggesting the fast cell internalization of these micelles. The similar phenomenon might be attributed to the biomimetic PMPC shell which was similar to the lipid bilayer and made it easily to be internalized by tumor cells, which was similar to with the work reported by Li’s group . Figure 4. View largeDownload slide 4T1 Uptake of free CDDP and CDDP-loaded micelles with the same concentration of pt. The data were presented as the average ± SD (n = 5) Figure 4. View largeDownload slide 4T1 Uptake of free CDDP and CDDP-loaded micelles with the same concentration of pt. The data were presented as the average ± SD (n = 5) The potential toxicity of PLG-b-PMPC block copolymer was first evaluated by MTT method against 4T1 cells. As shown in Fig. 5, the cell viability of 4T1 cells incubated with various concentration of PLG-b-PMPC was observed to be around 100% at all tests even at high concentration (100 µg/ml), indicating the excellent biocompatibility of PLG-b-PMPC. The great biocompatibility could be attributed to the zwitterionic PMPC shells of the micelles. The tumor cells inhibition efficacy of various concentrations of CDDP-loaded micelles was further evaluated against 4T1 cells after 48 and 72 h incubation, and free CDDP was used as control. As shown in Fig. 6, CDDP-loaded PLG-b-PMPC micelles exhibited similar inhibition efficiency with that of free CDDP at the same drug concentration after 48 and 72 h incubation. The result was consistent with the fast cell uptake behavior of the micelles (Fig. 4). Figure 5. View largeDownload slide Cell viability of 4T1 cells incubated with blank PLG-b-PMPC at various concentration. The data were presented as the average ± SD (n = 3) Figure 5. View largeDownload slide Cell viability of 4T1 cells incubated with blank PLG-b-PMPC at various concentration. The data were presented as the average ± SD (n = 3) Figure 6. View largeDownload slide In vitro cytotoxicity of CDDP-loaded micelles and free CDDP against 4T1 cells after 48 h (A) and 72 h (B). The data were presented as the average ± SD (n = 3) Figure 6. View largeDownload slide In vitro cytotoxicity of CDDP-loaded micelles and free CDDP against 4T1 cells after 48 h (A) and 72 h (B). The data were presented as the average ± SD (n = 3) Conclusions In this work, a CDDP loaded biomometic nanocarrier was prepared by complexation between CDDP and the carboxyl groups of hydrophilic PLG-b-PMPC copolymer with a desirable particle size of 91 nm and narrow size distribution. These CDDP-loaded polymeric micelles with the zwitterionic surface exhibited excellent stability in media containing proteins. CDDP was released from micelles in a sustained manner without the initial burst release and the drug release was faster in acidic condition due to the protonation of the carboxylic groups. Moreover, these biomimetic CDDP-loaded micelles exhibited similar cell uptake and tumor cells inhibition efficacy as free CDDP, indicating a promising micellar formulation incorporating CDDP for cancer therapy. Funding This research was supported by National Natural Science Foundation of China (Projects 51403131), Sichuan province Science-Technology Support Plan Project (2016SZ0004), the Programme of Introducing Talents of Discipline to Universities (B16033), and China Postdoctoral Science Foundation Funded Project (2015M570783). Conflict of interest statement. None declared. References 1 Arriagada R, Bergman B, Dunant A et al. Cisplatin-based adjuvant chemotherapy in patients with completely resected non-small-cell lung cancer. N Engl J Med 2004; 350: 351– 60. Google Scholar CrossRef Search ADS PubMed 2 Hartmann JT, Kollmannsberger C, Kanz L et al. Platinum organ toxicity and possible prevention in patients with testicular cancer. Int J Cancer 1999; 83: 866– 9. Google Scholar CrossRef Search ADS PubMed 3 Armstrong DK, Bundy B, Wenzel L et al. Intraperitoneal cisplatin and paclitaxel in ovarian cancer. N Engl J Med 2006; 354: 34– 43. Google Scholar CrossRef Search ADS PubMed 4 Iinuma H, Maruyama K, Okinaga K et al. Intracellular targeting therapy of cisplatin-encapsulated transferrin-polyethylene glycol liposome on peritoneal dissemination of gastric cancer. Int J Cancer 2002; 99: 130– 7. Google Scholar CrossRef Search ADS PubMed 5 Schlippe MV, Fowler CJ, Harland SJ. Cisplatin neurotoxicity in the treatment of metastatic germ cell tumour: Time course and prognosis. Br J Cancer 2001; 85: 823– 6. Google Scholar CrossRef Search ADS PubMed 6 Stewart DJ, Dulberg CS, Mikhael NZ et al. Association of cisplatin nephrotoxicity with patient characteristics and cisplatin administration methods. Cancer Chemother Pharmacol 1997; 40: 293– 308. Google Scholar CrossRef Search ADS PubMed 7 Cm WE. Giandomenico Current status of platinum-based antitumor drugs. Chem Rev 1999; 30: 2451– 66. 8 Butler JS, Sadler PJ. Targeted delivery of platinum-based anticancer complexes. Curr Opin Chem Biol 2013; 17: 175– 88. Google Scholar CrossRef Search ADS PubMed 9 Joaquim B, Antoni R, Natalia E et al. Carboplatin-based versus cisplatin-based chemotherapy in the treatment of surgically incurable advanced bladder carcinoma. Cancer 1997; 80: 1966– 72. Google Scholar CrossRef Search ADS PubMed 10 Ghorbani A, Omidvar B, Parsi A. Protective effect of selenium on cisplatin induced nephrotoxicity: a double-blind controlled randomized clinical trial. J Nephropathol 2013; 2: 129– 34. Google Scholar CrossRef Search ADS PubMed 11 Kidera Y, Kawakami H, Sakiyama T et al. Risk factors for cisplatin-induced nephrotoxicity and potential of magnesium supplementation for renal protection. PloS One 2014; 9: e101902. Google Scholar CrossRef Search ADS PubMed 12 Petros RA, DeSimone JM. Strategies in the design of nanoparticles for therapeutic applications. Nat Rev Drug Discov 2010; 9: 615– 27. Google Scholar CrossRef Search ADS PubMed 13 Fang J, Nakamura H, Maeda H. The EPR effect: Unique features of tumor blood vessels for drug delivery, factors involved, and limitations and augmentation of the effect. Adv Drug Deliv Rev 2011; 63: 136– 51. Google Scholar CrossRef Search ADS PubMed 14 Liu RY, Li Y, Zhang ZZ et al. Drug carriers based on highly protein-resistant materials for prolonged in vivo circulation time. Regen Biomater 2015; 2: 125– 33. Google Scholar CrossRef Search ADS PubMed 15 Kataoka K, Harada A, Nagasaki Y. Block copolymer micelles for drug delivery: design, characterization and biological significance. Adv Drug Deliv Rev 2001; 47: 113– 31. Google Scholar CrossRef Search ADS PubMed 16 Oberoi HS, Nukolova NV, Kabanov AV et al. Nanocarriers for delivery of platinum anticancer drugs. Adv Drug Deliv Rev 2013; 65: 1667– 85. Google Scholar CrossRef Search ADS PubMed 17 Cabral H, Kataoka K. Progress of drug-loaded polymeric micelles into clinical studies. J Control Release 2014; 190: 465– 76. Google Scholar CrossRef Search ADS PubMed 18 Uchino H, Matsumura Y, Negishi T et al. Cisplatin-incorporating polymeric micelles (NC-6004) can reduce nephrotoxicity and neurotoxicity of cisplatin in rats. Br J Cancer 2005; 93: 678– 87. Google Scholar CrossRef Search ADS PubMed 19 Nishiyama N, Kato Y, Sugiyama Y et al. Cisplatin-loaded polymer-metal complex micelle with time-modulated decaying property as a novel drug delivery system. Pharm Res 2001; 18: 1035– 41. Google Scholar CrossRef Search ADS PubMed 20 Yokoyama M, Okano T, Sakurai Y et al. Introduction of cisplatin into polymeric micelle. J Control Release 1996; 39: 351– 6. Google Scholar CrossRef Search ADS 21 Baba M, Matsumoto Y, Kashio A et al. Micellization of cisplatin (NC-6004) reduces its ototoxicity in guinea pigs. J Control Release 2012; 157: 112– 7. Google Scholar CrossRef Search ADS PubMed 22 Nishiyama N, Okazaki S, Cabral H et al. Novel cisplatin-incorporated polymeric micelles can eradicate solid tumors in mice. Cancer Res 2003; 63: 8977– 83. Google Scholar PubMed 23 Hadjichristidis N, Iatrou H, Pitsikalis M et al. Synthesis of well-defined polypeptide-based materials via the ring-opening polymerization of α-amino acid N-carboxyanhydrides. Chem Rev 2009; 109: 5528. Google Scholar CrossRef Search ADS PubMed 24 Amoozgar Z, Yeo Y. Recent advances in stealth coating of nanoparticle drug delivery systems. Wiley Interdiscip Rev Nanomed Nanobiotechnol 2012; 4: 219– 33. Google Scholar CrossRef Search ADS PubMed 25 Veronese FM, Pasut G. PEGylation, successful approach to drug delivery. Drug Discov Today 2005; 10: 1451–5 8. Google Scholar CrossRef Search ADS PubMed 26 Chaudhari KR, Ukawala M, Manjappa AS et al. Opsonization, biodistribution, cellular uptake and apoptosis study of PEGylated PBCA nanoparticle as potential drug delivery carrier. Pharm Res 2012; 29: 53– 68. Google Scholar CrossRef Search ADS PubMed 27 Cai TT, Lei Q, Yang B et al. Utilization of H-bond interaction of nucleobase Uralic with antitumor methotrexate to design drug carrier with ultrahigh loading efficiency and pH-responsive drug release. Regen Biomater 2014; 1: 27– 35. Google Scholar CrossRef Search ADS PubMed 28 Lobb EJ, Ma I, Billingham NC et al. Facile synthesis of well-defined, biocompatible phosphorylcholine-based methacrylate copolymers via atom transfer radical polymerization at 20 degrees °C. J Am Chem Soc 2001; 123: 7913– 4. Google Scholar CrossRef Search ADS PubMed 29 Monge S, Canniccioni B, Graillot A et al. Phosphorus-containing polymers: a great opportunity for the biomedical field. Biomacromolecules 2011; 12: 1973– 82. Google Scholar CrossRef Search ADS PubMed 30 Chantasirichot S, Inoue Y, Ishihara K. Amphiphilic triblock phospholipid copolymers bearing phenylboronic acid groups for spontaneous formation of hydrogels with tunable mechanical properties. Macromolecules 2014; 47: 3128– 35. Google Scholar CrossRef Search ADS 31 Liu GY, Chen CJ, Ji J. Biocompatible and biodegradable polymersomes as delivery vehicles in biomedical applications. Soft Matter 2012; 8: 8811. Google Scholar CrossRef Search ADS 32 Du JZ, Tang YQ, Lewis AL et al. pH-sensitive vesicles based on a biocompatible zwitterionic diblock copolymer. J Am Chem Soc 2005; 127: 17982– 3. Google Scholar CrossRef Search ADS PubMed 33 Sugihara S, Blanazs A, Armes SP et al. Aqueous dispersion polymerization: a new paradigm for in situ block copolymer self-assembly in concentrated solution. J Am Chem Soc 2011; 133: 15707– 13. Google Scholar CrossRef Search ADS PubMed 34 Liu GY, Jin Q, Liu XSg et al. Biocompatible vesicles based on PEO-b-PMPC/α-cyclodextrin inclusion complexes for drug delivery. Soft Matter 2011; 7: 662– 9. Google Scholar CrossRef Search ADS 35 Lomas H, Massignani M, Abdullah KA et al. Non-cytotoxic polymer vesicles for rapid and efficient intracellular delivery. Faraday Discuss 2008; 139: 143. Google Scholar CrossRef Search ADS PubMed 36 Wen YT, Zhang ZX, Li J. Highly Efficient multifunctional supramolecular gene carrier system self-assembled from redox-sensitive and zwitterionic polymer blocks. Adv Funct Mater 2014; 24: 3874– 84. Google Scholar CrossRef Search ADS 37 Liu GY, Zhuang WH, Chen XB et al. Drug carrier system self-assembled from biomimetic polyphosphorycholine and biodegradable polypeptide based diblock copolymers. Polymer 2016; 100: 45– 55. Google Scholar CrossRef Search ADS 38 Miyata K, Christie RJ, Kataoka K. Polymeric micelles for nano-scale drug delivery. React Funct Polym 2011; 71: 227– 34. Google Scholar CrossRef Search ADS © The Author(s) 2017. Published by Oxford University Press. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted reuse, distribution, and reproduction in any medium, provided the original work is properly cited.
Regenerative Biomaterials – Oxford University Press
Published: Feb 1, 2018
It’s your single place to instantly
discover and read the research
that matters to you.
Enjoy affordable access to
over 12 million articles from more than
10,000 peer-reviewed journals.
All for just $49/month
Read as many articles as you need. Full articles with original layout, charts and figures. Read online, from anywhere.
Keep up with your field with Personalized Recommendations and Follow Journals to get automatic updates.
It’s easy to organize your research with our built-in tools.
Read from thousands of the leading scholarly journals from SpringerNature, Elsevier, Wiley-Blackwell, Oxford University Press and more.
All the latest content is available, no embargo periods.
“Hi guys, I cannot tell you how much I love this resource. Incredible. I really believe you've hit the nail on the head with this site in regards to solving the research-purchase issue.”Daniel C.
“Whoa! It’s like Spotify but for academic articles.”@Phil_Robichaud
“I must say, @deepdyve is a fabulous solution to the independent researcher's problem of #access to #information.”@deepthiw
“My last article couldn't be possible without the platform @deepdyve that makes journal papers cheaper.”@JoseServera